 
data_c
 
_audit_creation_method            'SHELXL-2014/7'
_shelx_SHELXL_version_number      '2014/7'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          'Li0.16 Mg4 O32 Si7.84, 12(Ca)'
_chemical_formula_sum
 'Ca12 Li0.16 Mg4 O32 Si7.84' 
_chemical_formula_weight          1311.62

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mg'  'Mg'   0.0486   0.0363
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.0817   0.0704
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.2262   0.3064
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Li'  'Li'  -0.0003   0.0001
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       monoclinic
_space_group_IT_number            14
_space_group_name_H-M_alt         'P 21/c'
_space_group_name_Hall            '-P 2ybc'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _symmetry_equiv_pos_as_xyz 
 'x, y, z'
 '-x, y+1/2, -z+1/2'
 '-x, -y, -z'
 'x, -y-1/2, z-1/2'
 
_cell_length_a                    9.3416(4)
_cell_length_b                    5.3045(3)
_cell_length_c                    13.2848(7)
_cell_angle_alpha                 90
_cell_angle_beta                  92.088(2)
_cell_angle_gamma                 90
_cell_volume                      657.86(6)
_cell_formula_units_Z             1
_cell_measurement_temperature     273(2)
_cell_measurement_reflns_used     24619
_cell_measurement_theta_min       3.069 
_cell_measurement_theta_max       27.557
 
_exptl_crystal_description        block
_exptl_crystal_colour             colourless
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     3.337          
_exptl_crystal_F_000              659
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.04
_exptl_crystal_size_mid           0.03
_exptl_crystal_size_min           0.02
_exptl_absorpt_coefficient_mu     2.981
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_correction_T_min   0.6841
_exptl_absorpt_correction_T_max   0.7456
_exptl_absorpt_process_details  
;
SADABS-2004/1. Bruker AXS Inc., Madison, Wisconsin, USA, 2004
; 
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       273(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    ?
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean  ?
_diffrn_reflns_number             24619
_diffrn_reflns_av_unetI/netI      0.0223
_diffrn_reflns_av_R_equivalents   0.0564
_diffrn_reflns_limit_h_min        -12
_diffrn_reflns_limit_h_max        12
_diffrn_reflns_limit_k_min        -6
_diffrn_reflns_limit_k_max        6
_diffrn_reflns_limit_l_min        -17
_diffrn_reflns_limit_l_max        17
_diffrn_reflns_theta_min          3.069
_diffrn_reflns_theta_max          27.557
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.999
_diffrn_measured_fraction_theta_full  0.999
_diffrn_reflns_Laue_measured_fraction_max    0.999
_diffrn_reflns_Laue_measured_fraction_full   0.999
_diffrn_reflns_point_group_measured_fraction_max   0.999
_diffrn_reflns_point_group_measured_fraction_full  0.999
_reflns_number_total              1509
_reflns_number_gt                 1366
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        'APEX2 (Bruker, 2003-2008)' 
_computing_cell_refinement        'APEX2 (Bruker, 2003-2008)' 
_computing_data_reduction         'SAINT (Bruker, 2009)' 
_computing_structure_solution     'SHELXS-2014 (Sheldrick, 2014)'
_computing_structure_refinement   'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics     'DIAMOND (Brandenburg, 2005)' 
_computing_publication_material   'publCIF (Westrip, 2009)' 
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0532P)²+0.4782P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_extinction_coef        0.0023(8)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_number_reflns          1509
_refine_ls_number_parameters      130
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0343
_refine_ls_R_factor_gt            0.0295
_refine_ls_wR_factor_ref          0.0811
_refine_ls_wR_factor_gt           0.0780
_refine_ls_goodness_of_fit_ref    1.064
_refine_ls_restrained_S_all       1.064
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ca1 Ca 0.07532(5) 0.22717(9) 0.91873(4) 0.01074(16) Uani 1 1 d . . . . .
Ca2 Ca 0.77479(5) 0.17888(9) 0.74409(3) 0.01049(16) Uani 1 1 d . . . . .
Ca3 Ca 0.57485(5) 0.73283(9) 0.90277(4) 0.01168(16) Uani 1 1 d . . . . .
Mg Mg 0.25314(7) 0.75648(12) 0.50395(5) 0.0066(2) Uani 1 1 d . . . . .
Si1 Si 0.09329(6) 0.22784(11) 0.64126(5) 0.0045(2) Uani 0.982(4) 1 d . . P . .
Li1 Li 0.09329(6) 0.22784(11) 0.64126(5) 0.0045(2) Uani 0.018(4) 1 d . . P . .
Si2 Si 0.60032(6) 0.72921(11) 0.63311(5) 0.0048(2) Uani 0.979(4) 1 d . . P . .
Li2 Li 0.60032(6) 0.72921(11) 0.63311(5) 0.0048(2) Uani 0.021(4) 1 d . . P . .
O1 O 0.17516(16) 0.4571(3) 0.58305(12) 0.0119(4) Uani 1 1 d . . . . .
O2 O 0.67721(16) 0.4539(3) 0.62521(11) 0.0102(4) Uani 1 1 d . . . . .
O3 O 0.69356(16) 0.9205(3) 0.56439(12) 0.0133(4) Uani 1 1 d . . . . .
O4 O 0.18465(16) -0.0276(3) 0.62678(11) 0.0099(4) Uani 1 1 d . . . . .
O5 O -0.05896(16) 0.2057(3) 0.57696(12) 0.0129(4) Uani 1 1 d . . . . .
O6 O 0.06909(17) 0.3135(3) 0.75463(12) 0.0111(4) Uani 1 1 d . . . . .
O7 O 0.44529(17) 0.7124(3) 0.57401(13) 0.0147(4) Uani 1 1 d . . . . .
O8 O 0.59355(17) 0.8594(3) 0.74151(12) 0.0129(4) Uani 1 1 d . . . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ca1 O6 2.2264(17) . ?
Ca1 O3 2.3933(17) 2_646 ?
Ca1 O5 2.5121(17) 4_566 ?
Ca1 O1 2.5381(16) 4_566 ?
Ca1 O5 2.5439(18) 2_556 ?
Ca1 O1 2.7430(17) 2_546 ?
Ca1 O5 2.7708(18) 2_546 ?
Ca1 O4 2.8014(16) 2_556 ?
Ca1 O2 2.8080(16) 2_646 ?
Ca1 Li1 2.9646(8) 4_566 ?
Ca1 Si1 2.9646(8) 4_566 ?
Ca1 Li2 3.1318(7) 2_646 ?
Ca2 O2 2.3127(16) . ?
Ca2 O4 2.3373(16) 2_656 ?
Ca2 O8 2.3949(17) 1_545 ?
Ca2 O6 2.4250(17) 2_646 ?
Ca2 O1 2.6073(16) 2_646 ?
Ca2 O5 2.7592(17) 1_655 ?
Ca2 O3 2.8322(17) 1_545 ?
Ca2 O6 2.8390(17) 1_655 ?
Ca2 Li1 3.0701(8) 2_646 ?
Ca2 Si1 3.0701(8) 2_646 ?
Ca2 Li2 3.2163(8) 1_545 ?
Ca2 Si2 3.2163(8) 1_545 ?
Ca3 O8 2.2578(17) . ?
Ca3 O3 2.5155(17) 4_576 ?
Ca3 O7 2.5705(18) 2_656 ?
Ca3 O1 2.6215(16) 2_656 ?
Ca3 O7 2.6315(19) 4_576 ?
Ca3 O2 2.6445(16) 2_656 ?
Ca3 O4 2.6785(16) 2_656 ?
Ca3 O7 2.7847(18) 2_646 ?
Ca3 O3 3.0499(17) 2_646 ?
Ca3 Li2 3.0672(8) 4_576 ?
Ca3 Si2 3.0672(8) 4_576 ?
Ca3 Li2 3.1274(8) 2_656 ?
Mg O7 2.0052(17) . ?
Mg O3 2.0102(17) 3_676 ?
Mg O1 2.0526(17) . ?
Mg O5 2.0841(17) 3_566 ?
Mg O4 2.1118(17) 1_565 ?
Mg O2 2.1665(17) 3_666 ?
Mg Ca3 3.2183(8) 2_656 ?
Mg Ca1 3.2382(8) 4_565 ?
Mg Ca1 3.2747(8) 2_556 ?
Mg Ca2 3.3137(8) 3_666 ?
Mg Ca3 3.3370(9) 4_575 ?
Mg Ca1 3.3773(8) 4_575 ?
Si1 O6 1.5971(16) . ?
Si1 O4 1.6166(16) . ?
Si1 O5 1.6364(17) . ?
Si1 O1 1.6445(17) . ?
Si1 Ca1 2.9646(8) 4_565 ?
Si1 Ca2 3.0701(8) 2_656 ?
Si1 Ca1 3.1686(7) 2_556 ?
Si1 Ca1 3.1746(7) 2_546 ?
Si1 Ca3 3.1758(8) 2_646 ?
Si1 Ca2 3.3290(8) 1_455 ?
Si1 Ca2 3.4902(8) 2_646 ?
Si2 O8 1.6004(17) . ?
Si2 O7 1.6245(17) . ?
Si2 O2 1.6326(16) . ?
Si2 O3 1.6369(17) . ?
Si2 Ca3 3.0672(8) 4_575 ?
Si2 Ca3 3.1274(8) 2_646 ?
Si2 Ca1 3.1318(7) 2_656 ?
Si2 Ca3 3.1599(8) 2_656 ?
Si2 Ca2 3.2163(8) 1_565 ?
O1 Ca1 2.5381(16) 4_565 ?
O1 Ca2 2.6073(16) 2_656 ?
O1 Ca3 2.6215(16) 2_646 ?
O1 Ca1 2.7430(16) 2_556 ?
O2 Mg 2.1666(17) 3_666 ?
O2 Ca3 2.6446(16) 2_646 ?
O2 Ca1 2.8080(16) 2_656 ?
O3 Mg 2.0102(17) 3_676 ?
O3 Ca1 2.3934(16) 2_656 ?
O3 Ca3 2.5155(17) 4_575 ?
O3 Ca2 2.8322(17) 1_565 ?
O3 Ca3 3.0499(17) 2_656 ?
O4 Mg 2.1118(17) 1_545 ?
O4 Ca2 2.3373(16) 2_646 ?
O4 Ca3 2.6785(16) 2_646 ?
O4 Ca1 2.8014(16) 2_546 ?
O5 Mg 2.0842(17) 3_566 ?
O5 Ca1 2.5121(17) 4_565 ?
O5 Ca1 2.5440(18) 2_546 ?
O5 Ca2 2.7592(17) 1_455 ?
O5 Ca1 2.7708(18) 2_556 ?
O6 Ca2 2.4250(17) 2_656 ?
O6 Ca2 2.8390(17) 1_455 ?
O7 Ca3 2.5705(18) 2_646 ?
O7 Ca3 2.6315(19) 4_575 ?
O7 Ca3 2.7847(18) 2_656 ?
O8 Ca2 2.3949(17) 1_565 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O6 Ca1 O3 89.71(6) . 2_646 ?
O6 Ca1 O5 142.58(6) . 4_566 ?
O3 Ca1 O5 109.70(5) 2_646 4_566 ?
O6 Ca1 O1 156.51(6) . 4_566 ?
O3 Ca1 O1 77.43(5) 2_646 4_566 ?
O5 Ca1 O1 60.92(5) 4_566 4_566 ?
O6 Ca1 O5 79.47(6) . 2_556 ?
O3 Ca1 O5 67.98(5) 2_646 2_556 ?
O5 Ca1 O5 78.91(6) 4_566 2_556 ?
O1 Ca1 O5 112.67(6) 4_566 2_556 ?
O6 Ca1 O1 96.15(6) . 2_546 ?
O3 Ca1 O1 172.28(6) 2_646 2_546 ?
O5 Ca1 O1 68.25(5) 4_566 2_546 ?
O1 Ca1 O1 95.33(5) 4_566 2_546 ?
O5 Ca1 O1 118.00(5) 2_556 2_546 ?
O6 Ca1 O5 103.07(6) . 2_546 ?
O3 Ca1 O5 118.42(5) 2_646 2_546 ?
O5 Ca1 O5 95.42(5) 4_566 2_546 ?
O1 Ca1 O5 67.46(5) 4_566 2_546 ?
O5 Ca1 O5 172.86(7) 2_556 2_546 ?
O1 Ca1 O5 55.33(5) 2_546 2_546 ?
O6 Ca1 O4 72.64(5) . 2_556 ?
O3 Ca1 O4 126.39(5) 2_646 2_556 ?
O5 Ca1 O4 70.09(5) 4_566 2_556 ?
O1 Ca1 O4 130.76(5) 4_566 2_556 ?
O5 Ca1 O4 59.28(5) 2_556 2_556 ?
O1 Ca1 O4 60.54(5) 2_546 2_556 ?
O5 Ca1 O4 114.83(5) 2_546 2_556 ?
O6 Ca1 O2 83.97(5) . 2_646 ?
O3 Ca1 O2 59.60(5) 2_646 2_646 ?
O5 Ca1 O2 133.40(5) 4_566 2_646 ?
O1 Ca1 O2 72.57(5) 4_566 2_646 ?
O5 Ca1 O2 124.78(5) 2_556 2_646 ?
O1 Ca1 O2 115.92(5) 2_546 2_646 ?
O5 Ca1 O2 62.32(5) 2_546 2_646 ?
O4 Ca1 O2 155.32(5) 2_556 2_646 ?
O6 Ca1 Li1 163.42(5) . 4_566 ?
O3 Ca1 Li1 81.60(4) 2_646 4_566 ?
O5 Ca1 Li1 33.49(4) 4_566 4_566 ?
O1 Ca1 Li1 33.66(4) 4_566 4_566 ?
O5 Ca1 Li1 84.17(4) 2_556 4_566 ?
O1 Ca1 Li1 93.90(4) 2_546 4_566 ?
O5 Ca1 Li1 93.49(4) 2_546 4_566 ?
O4 Ca1 Li1 101.24(4) 2_556 4_566 ?
O2 Ca1 Li1 103.40(4) 2_646 4_566 ?
O6 Ca1 Si1 163.42(5) . 4_566 ?
O3 Ca1 Si1 81.60(4) 2_646 4_566 ?
O5 Ca1 Si1 33.49(4) 4_566 4_566 ?
O1 Ca1 Si1 33.66(4) 4_566 4_566 ?
O5 Ca1 Si1 84.17(4) 2_556 4_566 ?
O1 Ca1 Si1 93.90(4) 2_546 4_566 ?
O5 Ca1 Si1 93.49(4) 2_546 4_566 ?
O4 Ca1 Si1 101.24(4) 2_556 4_566 ?
O2 Ca1 Si1 103.40(4) 2_646 4_566 ?
Li1 Ca1 Si1 0.0 4_566 4_566 ?
O6 Ca1 Li2 76.99(4) . 2_646 ?
O3 Ca1 Li2 30.95(4) 2_646 2_646 ?
O5 Ca1 Li2 134.44(4) 4_566 2_646 ?
O1 Ca1 Li2 82.09(4) 4_566 2_646 ?
O5 Ca1 Li2 93.49(4) 2_556 2_646 ?
O1 Ca1 Li2 146.28(4) 2_546 2_646 ?
O5 Ca1 Li2 93.58(4) 2_546 2_646 ?
O4 Ca1 Li2 142.09(4) 2_556 2_646 ?
O2 Ca1 Li2 31.30(3) 2_646 2_646 ?
Li1 Ca1 Li2 101.47(2) 4_566 2_646 ?
Si1 Ca1 Li2 101.47(2) 4_566 2_646 ?
O2 Ca2 O4 97.49(6) . 2_656 ?
O2 Ca2 O8 100.12(6) . 1_545 ?
O4 Ca2 O8 125.27(6) 2_656 1_545 ?
O2 Ca2 O6 136.96(6) . 2_646 ?
O4 Ca2 O6 116.47(6) 2_656 2_646 ?
O8 Ca2 O6 81.91(6) 1_545 2_646 ?
O2 Ca2 O1 160.00(6) . 2_646 ?
O4 Ca2 O1 68.60(5) 2_656 2_646 ?
O8 Ca2 O1 78.30(5) 1_545 2_646 ?
O6 Ca2 O1 62.92(5) 2_646 2_646 ?
O2 Ca2 O5 68.73(5) . 1_655 ?
O4 Ca2 O5 118.38(5) 2_656 1_655 ?
O8 Ca2 O5 116.32(5) 1_545 1_655 ?
O6 Ca2 O5 72.00(5) 2_646 1_655 ?
O1 Ca2 O5 130.08(5) 2_646 1_655 ?
O2 Ca2 O3 69.07(5) . 1_545 ?
O4 Ca2 O3 166.48(6) 2_656 1_545 ?
O8 Ca2 O3 58.53(5) 1_545 1_545 ?
O6 Ca2 O3 76.22(5) 2_646 1_545 ?
O1 Ca2 O3 123.91(6) 2_646 1_545 ?
O5 Ca2 O3 59.21(5) 1_655 1_545 ?
O2 Ca2 O6 103.41(5) . 1_655 ?
O4 Ca2 O6 70.45(5) 2_656 1_655 ?
O8 Ca2 O6 149.50(6) 1_545 1_655 ?
O6 Ca2 O6 67.65(3) 2_646 1_655 ?
O1 Ca2 O6 85.86(5) 2_646 1_655 ?
O5 Ca2 O6 56.93(5) 1_655 1_655 ?
O3 Ca2 O6 113.11(5) 1_545 1_655 ?
O2 Ca2 Li1 166.28(5) . 2_646 ?
O4 Ca2 Li1 95.95(4) 2_656 2_646 ?
O8 Ca2 Li1 74.12(4) 1_545 2_646 ?
O6 Ca2 Li1 31.06(4) 2_646 2_646 ?
O1 Ca2 Li1 32.39(4) 2_646 2_646 ?
O5 Ca2 Li1 102.24(4) 1_655 2_646 ?
O3 Ca2 Li1 97.55(4) 1_545 2_646 ?
O6 Ca2 Li1 78.53(4) 1_655 2_646 ?
O2 Ca2 Si1 166.28(5) . 2_646 ?
O4 Ca2 Si1 95.95(4) 2_656 2_646 ?
O8 Ca2 Si1 74.12(4) 1_545 2_646 ?
O6 Ca2 Si1 31.06(4) 2_646 2_646 ?
O1 Ca2 Si1 32.39(4) 2_646 2_646 ?
O5 Ca2 Si1 102.24(4) 1_655 2_646 ?
O3 Ca2 Si1 97.55(4) 1_545 2_646 ?
O6 Ca2 Si1 78.53(4) 1_655 2_646 ?
Li1 Ca2 Si1 0.0 2_646 2_646 ?
O2 Ca2 Li2 88.52(4) . 1_545 ?
O4 Ca2 Li2 153.68(4) 2_656 1_545 ?
O8 Ca2 Li2 28.65(4) 1_545 1_545 ?
O6 Ca2 Li2 72.85(4) 2_646 1_545 ?
O1 Ca2 Li2 98.09(4) 2_646 1_545 ?
O5 Ca2 Li2 87.71(4) 1_655 1_545 ?
O3 Ca2 Li2 30.57(3) 1_545 1_545 ?
O6 Ca2 Li2 133.07(4) 1_655 1_545 ?
Li1 Ca2 Li2 80.62(2) 2_646 1_545 ?
Si1 Ca2 Li2 80.62(2) 2_646 1_545 ?
O2 Ca2 Si2 88.52(4) . 1_545 ?
O4 Ca2 Si2 153.68(4) 2_656 1_545 ?
O8 Ca2 Si2 28.65(4) 1_545 1_545 ?
O6 Ca2 Si2 72.85(4) 2_646 1_545 ?
O1 Ca2 Si2 98.09(4) 2_646 1_545 ?
O5 Ca2 Si2 87.71(4) 1_655 1_545 ?
O3 Ca2 Si2 30.57(3) 1_545 1_545 ?
O6 Ca2 Si2 133.07(4) 1_655 1_545 ?
Li1 Ca2 Si2 80.62(2) 2_646 1_545 ?
Si1 Ca2 Si2 80.62(2) 2_646 1_545 ?
Li2 Ca2 Si2 0.0 1_545 1_545 ?
O8 Ca3 O3 149.21(6) . 4_576 ?
O8 Ca3 O7 80.10(6) . 2_656 ?
O3 Ca3 O7 104.45(6) 4_576 2_656 ?
O8 Ca3 O1 80.43(6) . 2_656 ?
O3 Ca3 O1 73.83(5) 4_576 2_656 ?
O7 Ca3 O1 67.12(5) 2_656 2_656 ?
O8 Ca3 O7 147.28(6) . 4_576 ?
O3 Ca3 O7 60.01(5) 4_576 4_576 ?
O7 Ca3 O7 75.47(6) 2_656 4_576 ?
O1 Ca3 O7 108.93(5) 2_656 4_576 ?
O8 Ca3 O2 80.45(5) . 2_656 ?
O3 Ca3 O2 128.75(5) 4_576 2_656 ?
O7 Ca3 O2 60.62(5) 2_656 2_656 ?
O1 Ca3 O2 126.53(5) 2_656 2_656 ?
O7 Ca3 O2 68.74(5) 4_576 2_656 ?
O8 Ca3 O4 85.41(6) . 2_656 ?
O3 Ca3 O4 67.19(5) 4_576 2_656 ?
O7 Ca3 O4 126.41(5) 2_656 2_656 ?
O1 Ca3 O4 59.65(5) 2_656 2_656 ?
O7 Ca3 O4 126.74(5) 4_576 2_656 ?
O2 Ca3 O4 162.82(6) 2_656 2_656 ?
O8 Ca3 O7 114.06(6) . 2_646 ?
O3 Ca3 O7 67.32(5) 4_576 2_646 ?
O7 Ca3 O7 164.21(8) 2_656 2_646 ?
O1 Ca3 O7 120.36(5) 2_656 2_646 ?
O7 Ca3 O7 88.77(6) 4_576 2_646 ?
O2 Ca3 O7 113.06(5) 2_656 2_646 ?
O4 Ca3 O7 64.24(5) 2_656 2_646 ?
O8 Ca3 O3 112.94(5) . 2_646 ?
O3 Ca3 O3 92.37(5) 4_576 2_646 ?
O7 Ca3 O3 117.15(5) 2_656 2_646 ?
O1 Ca3 O3 166.19(5) 2_656 2_646 ?
O7 Ca3 O3 61.96(5) 4_576 2_646 ?
O2 Ca3 O3 61.87(5) 2_656 2_646 ?
O4 Ca3 O3 116.05(5) 2_656 2_646 ?
O7 Ca3 O3 52.15(5) 2_646 2_646 ?
O8 Ca3 Li2 157.10(5) . 4_576 ?
O3 Ca3 Li2 32.21(4) 4_576 4_576 ?
O7 Ca3 Li2 79.55(4) 2_656 4_576 ?
O1 Ca3 Li2 82.07(4) 2_656 4_576 ?
O7 Ca3 Li2 31.97(4) 4_576 4_576 ?
O2 Ca3 Li2 98.48(4) 2_656 4_576 ?
O4 Ca3 Li2 98.34(4) 2_656 4_576 ?
O7 Ca3 Li2 87.57(4) 2_646 4_576 ?
O3 Ca3 Li2 85.83(3) 2_646 4_576 ?
O8 Ca3 Si2 157.10(5) . 4_576 ?
O3 Ca3 Si2 32.21(4) 4_576 4_576 ?
O7 Ca3 Si2 79.55(4) 2_656 4_576 ?
O1 Ca3 Si2 82.07(4) 2_656 4_576 ?
O7 Ca3 Si2 31.97(4) 4_576 4_576 ?
O2 Ca3 Si2 98.48(4) 2_656 4_576 ?
O4 Ca3 Si2 98.34(4) 2_656 4_576 ?
O7 Ca3 Si2 87.57(4) 2_646 4_576 ?
O3 Ca3 Si2 85.83(3) 2_646 4_576 ?
Li2 Ca3 Si2 0.0 4_576 4_576 ?
O8 Ca3 Li2 70.32(5) . 2_656 ?
O3 Ca3 Li2 127.89(4) 4_576 2_656 ?
O7 Ca3 Li2 31.22(4) 2_656 2_656 ?
O1 Ca3 Li2 95.09(4) 2_656 2_656 ?
O7 Ca3 Li2 77.54(4) 4_576 2_656 ?
O2 Ca3 Li2 31.46(4) 2_656 2_656 ?
O4 Ca3 Li2 148.09(4) 2_656 2_656 ?
O7 Ca3 Li2 144.53(4) 2_646 2_656 ?
O3 Ca3 Li2 92.92(3) 2_646 2_656 ?
Li2 Ca3 Li2 96.77(2) 4_576 2_656 ?
Si2 Ca3 Li2 96.77(2) 4_576 2_656 ?
O7 Mg O3 94.40(7) . 3_676 ?
O7 Mg O1 90.03(7) . . ?
O3 Mg O1 171.53(7) 3_676 . ?
O7 Mg O5 176.48(7) . 3_566 ?
O3 Mg O5 84.86(7) 3_676 3_566 ?
O1 Mg O5 91.15(7) . 3_566 ?
O7 Mg O4 89.76(7) . 1_565 ?
O3 Mg O4 88.49(7) 3_676 1_565 ?
O1 Mg O4 84.31(7) . 1_565 ?
O5 Mg O4 93.66(7) 3_566 1_565 ?
O7 Mg O2 91.03(7) . 3_666 ?
O3 Mg O2 89.71(7) 3_676 3_666 ?
O1 Mg O2 97.43(7) . 3_666 ?
O5 Mg O2 85.52(7) 3_566 3_666 ?
O4 Mg O2 178.09(6) 1_565 3_666 ?
O7 Mg Ca3 59.12(5) . 2_656 ?
O3 Mg Ca3 51.41(5) 3_676 2_656 ?
O1 Mg Ca3 126.29(5) . 2_656 ?
O5 Mg Ca3 122.42(6) 3_566 2_656 ?
O4 Mg Ca3 55.79(5) 1_565 2_656 ?
O2 Mg Ca3 123.31(5) 3_666 2_656 ?
O7 Mg Ca1 120.60(6) . 4_565 ?
O3 Mg Ca1 130.53(5) 3_676 4_565 ?
O1 Mg Ca1 51.60(5) . 4_565 ?
O5 Mg Ca1 58.00(5) 3_566 4_565 ?
O4 Mg Ca1 122.26(5) 1_565 4_565 ?
O2 Mg Ca1 58.67(4) 3_666 4_565 ?
Ca3 Mg Ca1 177.76(3) 2_656 4_565 ?
O7 Mg Ca1 133.00(6) . 2_556 ?
O3 Mg Ca1 115.62(5) 3_676 2_556 ?
O1 Mg Ca1 56.54(5) . 2_556 ?
O5 Mg Ca1 50.10(5) 3_566 2_556 ?
O4 Mg Ca1 57.97(5) 1_565 2_556 ?
O2 Mg Ca1 122.40(5) 3_666 2_556 ?
Ca3 Mg Ca1 112.14(2) 2_656 2_556 ?
Ca1 Mg Ca1 66.262(19) 4_565 2_556 ?
O7 Mg Ca2 120.69(6) . 3_666 ?
O3 Mg Ca2 58.30(5) 3_676 3_666 ?
O1 Mg Ca2 124.93(5) . 3_666 ?
O5 Mg Ca2 56.06(5) 3_566 3_666 ?
O4 Mg Ca2 134.20(5) 1_565 3_666 ?
O2 Mg Ca2 44.02(4) 3_666 3_666 ?
Ca3 Mg Ca2 108.77(2) 2_656 3_666 ?
Ca1 Mg Ca2 73.355(18) 4_565 3_666 ?
Ca1 Mg Ca2 106.03(2) 2_556 3_666 ?
O7 Mg Ca3 52.04(5) . 4_575 ?
O3 Mg Ca3 64.03(5) 3_676 4_575 ?
O1 Mg Ca3 124.12(5) . 4_575 ?
O5 Mg Ca3 124.77(5) 3_566 4_575 ?
O4 Mg Ca3 127.20(5) 1_565 4_575 ?
O2 Mg Ca3 52.33(4) 3_666 4_575 ?
Ca3 Mg Ca3 72.39(2) 2_656 4_575 ?
Ca1 Mg Ca3 109.31(2) 4_565 4_575 ?
Ca1 Mg Ca3 174.28(3) 2_556 4_575 ?
Ca2 Mg Ca3 68.725(19) 3_666 4_575 ?
O7 Mg Ca1 132.15(6) . 4_575 ?
O3 Mg Ca1 44.29(5) 3_676 4_575 ?
O1 Mg Ca1 128.30(5) . 4_575 ?
O5 Mg Ca1 48.77(5) 3_566 4_575 ?
O4 Mg Ca1 70.12(5) 1_565 4_575 ?
O2 Mg Ca1 108.09(5) 3_666 4_575 ?
Ca3 Mg Ca1 74.032(19) 2_656 4_575 ?
Ca1 Mg Ca1 106.59(2) 4_565 4_575 ?
Ca1 Mg Ca1 71.857(19) 2_556 4_575 ?
Ca2 Mg Ca1 64.076(16) 3_666 4_575 ?
Ca3 Mg Ca1 106.88(2) 4_575 4_575 ?
O6 Si1 O4 116.38(9) . . ?
O6 Si1 O5 111.25(9) . . ?
O4 Si1 O5 109.29(9) . . ?
O6 Si1 O1 108.49(9) . . ?
O4 Si1 O1 107.89(9) . . ?
O5 Si1 O1 102.58(9) . . ?
O6 Si1 Ca1 155.87(7) . 4_565 ?
O4 Si1 Ca1 87.69(6) . 4_565 ?
O5 Si1 Ca1 57.90(6) . 4_565 ?
O1 Si1 Ca1 58.80(6) . 4_565 ?
O6 Si1 Ca2 51.57(6) . 2_656 ?
O4 Si1 Ca2 120.54(6) . 2_656 ?
O5 Si1 Ca2 129.82(7) . 2_656 ?
O1 Si1 Ca2 58.13(6) . 2_656 ?
Ca1 Si1 Ca2 116.05(3) 4_565 2_656 ?
O6 Si1 Ca1 85.02(6) . 2_556 ?
O4 Si1 Ca1 158.50(7) . 2_556 ?
O5 Si1 Ca1 60.92(6) . 2_556 ?
O1 Si1 Ca1 59.94(6) . 2_556 ?
Ca1 Si1 Ca1 70.87(2) 4_565 2_556 ?
Ca2 Si1 Ca1 70.138(17) 2_656 2_556 ?
O6 Si1 Ca1 112.89(6) . 2_546 ?
O4 Si1 Ca1 61.84(6) . 2_546 ?
O5 Si1 Ca1 52.78(6) . 2_546 ?
O1 Si1 Ca1 137.35(6) . 2_546 ?
Ca1 Si1 Ca1 78.90(2) 4_565 2_546 ?
Ca2 Si1 Ca1 164.37(3) 2_656 2_546 ?
Ca1 Si1 Ca1 113.49(2) 2_556 2_546 ?
O6 Si1 Ca3 110.12(6) . 2_646 ?
O4 Si1 Ca3 57.45(6) . 2_646 ?
O5 Si1 Ca3 137.74(7) . 2_646 ?
O1 Si1 Ca3 55.49(6) . 2_646 ?
Ca1 Si1 Ca3 80.55(2) 4_565 2_646 ?
Ca2 Si1 Ca3 73.023(18) 2_656 2_646 ?
Ca1 Si1 Ca3 115.23(2) 2_556 2_646 ?
Ca1 Si1 Ca3 116.07(2) 2_546 2_646 ?
O6 Si1 Ca2 58.39(6) . 1_455 ?
O4 Si1 Ca2 117.84(6) . 1_455 ?
O5 Si1 Ca2 55.65(6) . 1_455 ?
O1 Si1 Ca2 133.51(6) . 1_455 ?
Ca1 Si1 Ca2 113.36(2) 4_565 1_455 ?
Ca2 Si1 Ca2 101.88(2) 2_656 1_455 ?
Ca1 Si1 Ca2 74.034(17) 2_556 1_455 ?
Ca1 Si1 Ca2 66.114(16) 2_546 1_455 ?
Ca3 Si1 Ca2 165.76(3) 2_646 1_455 ?
O6 Si1 Ca2 83.45(6) . 2_646 ?
O4 Si1 Ca2 34.22(6) . 2_646 ?
O5 Si1 Ca2 117.02(7) . 2_646 ?
O1 Si1 Ca2 131.24(6) . 2_646 ?
Ca1 Si1 Ca2 120.57(2) 4_565 2_646 ?
Ca2 Si1 Ca2 107.74(2) 2_656 2_646 ?
Ca1 Si1 Ca2 166.31(2) 2_556 2_646 ?
Ca1 Si1 Ca2 64.889(16) 2_546 2_646 ?
Ca3 Si1 Ca2 75.867(18) 2_646 2_646 ?
Ca2 Si1 Ca2 93.58(2) 1_455 2_646 ?
O8 Si2 O7 113.25(9) . . ?
O8 Si2 O2 118.41(9) . . ?
O7 Si2 O2 107.85(9) . . ?
O8 Si2 O3 105.88(9) . . ?
O7 Si2 O3 104.33(9) . . ?
O2 Si2 O3 105.92(9) . . ?
O8 Si2 Ca3 149.91(7) . 4_575 ?
O7 Si2 Ca3 59.07(7) . 4_575 ?
O2 Si2 Ca3 90.74(6) . 4_575 ?
O3 Si2 Ca3 55.00(6) . 4_575 ?
O8 Si2 Ca3 117.57(7) . 2_646 ?
O7 Si2 Ca3 55.11(7) . 2_646 ?
O2 Si2 Ca3 57.73(6) . 2_646 ?
O3 Si2 Ca3 136.30(7) . 2_646 ?
Ca3 Si2 Ca3 83.23(2) 4_575 2_646 ?
O8 Si2 Ca1 105.64(6) . 2_656 ?
O7 Si2 Ca1 138.26(7) . 2_656 ?
O2 Si2 Ca1 63.34(6) . 2_656 ?
O3 Si2 Ca1 48.76(6) . 2_656 ?
Ca3 Si2 Ca1 79.71(2) 4_575 2_656 ?
Ca3 Si2 Ca1 117.94(2) 2_646 2_656 ?
O8 Si2 Ca3 74.56(6) . 2_656 ?
O7 Si2 Ca3 61.69(6) . 2_656 ?
O2 Si2 Ca3 166.71(6) . 2_656 ?
O3 Si2 Ca3 71.03(6) . 2_656 ?
Ca3 Si2 Ca3 76.88(2) 4_575 2_656 ?
Ca3 Si2 Ca3 115.06(2) 2_646 2_656 ?
Ca1 Si2 Ca3 118.01(2) 2_656 2_656 ?
O8 Si2 Ca2 45.85(6) . 1_565 ?
O7 Si2 Ca2 133.64(7) . 1_565 ?
O2 Si2 Ca2 118.43(6) . 1_565 ?
O3 Si2 Ca2 61.64(6) . 1_565 ?
Ca3 Si2 Ca2 115.36(2) 4_575 1_565 ?
Ca3 Si2 Ca2 161.41(3) 2_646 1_565 ?
Ca1 Si2 Ca2 67.987(16) 2_656 1_565 ?
Ca3 Si2 Ca2 72.130(18) 2_656 1_565 ?
O8 Si2 Ca3 25.29(6) . . ?
O7 Si2 Ca3 113.03(7) . . ?
O2 Si2 Ca3 96.54(6) . . ?
O3 Si2 Ca3 127.42(6) . . ?
Ca3 Si2 Ca3 170.81(3) 4_575 . ?
Ca3 Si2 Ca3 95.91(2) 2_646 . ?
Ca1 Si2 Ca3 108.57(2) 2_656 . ?
Ca3 Si2 Ca3 95.34(2) 2_656 . ?
Ca2 Si2 Ca3 65.828(16) 1_565 . ?
O8 Si2 Ca2 90.77(6) . . ?
O7 Si2 Ca2 122.10(7) . . ?
O2 Si2 Ca2 27.70(6) . . ?
O3 Si2 Ca2 119.00(6) . . ?
Ca3 Si2 Ca2 118.38(2) 4_575 . ?
Ca3 Si2 Ca2 67.016(17) 2_646 . ?
Ca1 Si2 Ca2 70.296(16) 2_656 . ?
Ca3 Si2 Ca2 164.48(2) 2_656 . ?
Ca2 Si2 Ca2 101.40(2) 1_565 . ?
Ca3 Si2 Ca2 69.206(15) . . ?
Si1 O1 Mg 173.05(10) . . ?
Si1 O1 Ca1 87.54(7) . 4_565 ?
Mg O1 Ca1 89.07(6) . 4_565 ?
Si1 O1 Ca2 89.49(7) . 2_656 ?
Mg O1 Ca2 92.65(6) . 2_656 ?
Ca1 O1 Ca2 168.45(7) 4_565 2_656 ?
Si1 O1 Ca3 93.38(7) . 2_646 ?
Mg O1 Ca3 93.21(6) . 2_646 ?
Ca1 O1 Ca3 100.69(6) 4_565 2_646 ?
Ca2 O1 Ca3 90.62(5) 2_656 2_646 ?
Si1 O1 Ca1 88.80(7) . 2_556 ?
Mg O1 Ca1 84.83(6) . 2_556 ?
Ca1 O1 Ca1 84.67(5) 4_565 2_556 ?
Ca2 O1 Ca1 84.12(5) 2_656 2_556 ?
Ca3 O1 Ca1 174.28(7) 2_646 2_556 ?
Si2 O2 Mg 131.09(9) . 3_666 ?
Si2 O2 Ca2 133.14(9) . . ?
Mg O2 Ca2 95.37(6) 3_666 . ?
Si2 O2 Ca3 90.81(7) . 2_646 ?
Mg O2 Ca3 87.24(6) 3_666 2_646 ?
Ca2 O2 Ca3 98.22(6) . 2_646 ?
Si2 O2 Ca1 85.36(7) . 2_656 ?
Mg O2 Ca1 80.10(5) 3_666 2_656 ?
Ca2 O2 Ca1 99.24(5) . 2_656 ?
Ca3 O2 Ca1 159.27(6) 2_646 2_656 ?
Si2 O3 Mg 157.79(11) . 3_676 ?
Si2 O3 Ca1 100.29(8) . 2_656 ?
Mg O3 Ca1 99.79(7) 3_676 2_656 ?
Si2 O3 Ca3 92.79(7) . 4_575 ?
Mg O3 Ca3 89.93(6) 3_676 4_575 ?
Ca1 O3 Ca3 108.03(6) 2_656 4_575 ?
Si2 O3 Ca2 87.80(7) . 1_565 ?
Mg O3 Ca2 84.55(6) 3_676 1_565 ?
Ca1 O3 Ca2 85.14(5) 2_656 1_565 ?
Ca3 O3 Ca2 166.45(7) 4_575 1_565 ?
Si2 O3 Ca3 78.46(6) . 2_656 ?
Mg O3 Ca3 79.63(6) 3_676 2_656 ?
Ca1 O3 Ca3 164.34(7) 2_656 2_656 ?
Ca3 O3 Ca3 87.63(5) 4_575 2_656 ?
Ca2 O3 Ca3 79.22(4) 1_565 2_656 ?
Si1 O4 Mg 136.28(9) . 1_545 ?
Si1 O4 Ca2 122.90(8) . 2_646 ?
Mg O4 Ca2 99.22(7) 1_545 2_646 ?
Si1 O4 Ca3 91.97(7) . 2_646 ?
Mg O4 Ca3 83.52(5) 1_545 2_646 ?
Ca2 O4 Ca3 109.68(6) 2_646 2_646 ?
Si1 O4 Ca1 87.57(6) . 2_546 ?
Mg O4 Ca1 82.30(5) 1_545 2_546 ?
Ca2 O4 Ca1 88.00(5) 2_646 2_546 ?
Ca3 O4 Ca1 158.91(6) 2_646 2_546 ?
Si1 O5 Mg 170.37(11) . 3_566 ?
Si1 O5 Ca1 88.61(7) . 4_565 ?
Mg O5 Ca1 90.38(6) 3_566 4_565 ?
Si1 O5 Ca1 96.40(8) . 2_546 ?
Mg O5 Ca1 93.19(6) 3_566 2_546 ?
Ca1 O5 Ca1 101.09(6) 4_565 2_546 ?
Si1 O5 Ca2 95.03(7) . 1_455 ?
Mg O5 Ca2 85.13(6) 3_566 1_455 ?
Ca1 O5 Ca2 173.46(7) 4_565 1_455 ?
Ca1 O5 Ca2 83.94(5) 2_546 1_455 ?
Si1 O5 Ca1 88.01(7) . 2_556 ?
Mg O5 Ca1 82.36(6) 3_566 2_556 ?
Ca1 O5 Ca1 84.57(5) 4_565 2_556 ?
Ca1 O5 Ca1 172.87(7) 2_546 2_556 ?
Ca2 O5 Ca1 90.11(5) 1_455 2_556 ?
Si1 O6 Ca1 149.91(10) . . ?
Si1 O6 Ca2 97.37(7) . 2_656 ?
Ca1 O6 Ca2 99.40(6) . 2_656 ?
Si1 O6 Ca2 92.98(7) . 1_455 ?
Ca1 O6 Ca2 89.27(5) . 1_455 ?
Ca2 O6 Ca2 141.49(7) 2_656 1_455 ?
Si2 O7 Mg 170.11(11) . . ?
Si2 O7 Ca3 93.67(8) . 2_646 ?
Mg O7 Ca3 95.90(7) . 2_646 ?
Si2 O7 Ca3 88.96(7) . 4_575 ?
Mg O7 Ca3 91.03(7) . 4_575 ?
Ca3 O7 Ca3 104.53(6) 2_646 4_575 ?
Si2 O7 Ca3 87.41(7) . 2_656 ?
Mg O7 Ca3 82.70(6) . 2_656 ?
Ca3 O7 Ca3 164.21(8) 2_646 2_656 ?
Ca3 O7 Ca3 91.23(6) 4_575 2_656 ?
Si2 O8 Ca3 137.09(10) . . ?
Si2 O8 Ca2 105.49(8) . 1_565 ?
Ca3 O8 Ca2 106.02(6) . 1_565 ?
 
_refine_diff_density_max    0.833
_refine_diff_density_min   -0.459
_refine_diff_density_rms    0.141



